**N A N O E X P R E S S**

**Open Access**

## Theoretical Investigation of Biaxially

## Tensile-Strained Germanium Nanowires

### Zhongyunshen Zhu

1,2### , Yuxin Song

1*### , Qimiao Chen

1,3### , Zhenpu Zhang

1,2### , Liyao Zhang

1### , Yaoyao Li

1### and Shumin Wang

1,4***Abstract**

We theoretically investigate highly tensile-strained Ge nanowires laterally on GaSb. Finite element method has been used to simulate the residual elastic strain in the Ge nanowire. The total energy increment including strain energy, surface energy, and edge energy before and after Ge deposition is calculated in different situations. The result indicates that the Ge nanowire on GaSb is apt to grow along100rather than110in the two situations and prefers to be exposed by{105}facets when deposited a small amount of Ge but to be exposed by{110}when the amount of Ge exceeds a critical value. Furthermore, the conduction band minima in-valley at any position in both situations exhibits lower values than those in L-valley, leading to direct bandgap transition in Ge nanowire. For the valence band, the light hole band maxima at-point is higher than the heavy hole band maxima at any position and even higher than the conduction band minima for the hydrostatic strain more than∼5.0%, leading to a negative bandgap. In addition, both electron and hole mobility can be enhanced by owing to the decrease of the effective mass under highly tensile strain. The results suggest that biaxially tensile-strained Ge nanowires hold promising properties in device applications.

**Keywords:** Tensile strain, Ge nanowire, Finite element method, Direct bandgap, Mobility

**Background**

As a group IV element, germanium (Ge) holds the
supe-riority both in optoelectronics and electronics and has
great compatibility with silicon (Si) photonics. An
essen-tial characteristic of Ge is that its direct bandgap is around
0.8 eV (1.55 *μ*m) at 300 K. The mobility of both
elec-tron and hole in Ge is much higher than that in Si. Thus,
Ge has been utilized in high speed devices in current
Si-based integrated circuit [1, 2]. More interestingly,
tensile-strained Ge offers optimization in the above aspects. Ge
is an indirect bandgap semiconductor with a slight
dif-ference of 136 meV between L-valley and-valley [3]. It
is theoretically predicted that over∼4.0% uniaxial along
111 [4] or ∼1.6–2.0% biaxial [5, 6] tensile strain can

*Correspondence: [email protected]; [email protected]

1_{State Key Laboratory of Functional Materials for Informatics, Shanghai}

Institute of Microsystem and Information Technology, Chinese Academy of Sciences, Shanghai 200050, China

4_{Department of Microtechnology and Nanoscience, Chalmers University of}

Technology, 41296 Gothenburg, Sweden

Full list of author information is available at the end of the article

lower the -valley below the L-valley, thereby convert-ing Ge into a direct bandgap material, which opens a new route for light emitting from group IV materials. Another important point is that tensile-strained Ge provides signif-icant enhancement in carrier mobility [7, 8] for realizing high speed complementary metal oxide semiconductor devices.

Nanowires (NWs) exhibit attractive electronic and
opti-cal properties owing to the large surface to volume ratio
and confinement of both carriers and photons in two
dimensions (2D) [9]. In the past years, Ge NWs (GeNWs)
on Si [10] or Ge/Si core/shell NWs [11] have been under
extensive study due to their potentials in metal oxide
semiconductor field-effect transistors (MOSFETs) for Si
microelectronics. Both the scaled transconductance and
on-current were enhanced by three to four times
com-pared with conventional Si*p*-MOSFET [12]. Thus,
epi-taxial growth of lateral GeNWs directly on Si has been
expected to fabricate high performance MOSFETs. Zhang
et al. addressed that ultrathin GeNWs on Si (001) are
exposed with facets of {105} [13], which have the
low-est predicted surface energy [14]. Further, strained Ge

MOSFET on SiGe virtual substrate was shown to improve the hole mobility [1]. Although lateral GeNW on Si with compressive strain can display significant improvement in carrier transport as assumed, they are unable to be con-verted into a direct bandgap. For introducing tensile strain in GeNWs, GeSn alloy [15] and III-Sb compounds [16], which have a larger lattice constant than that of Ge, are required. In spite of that mechanical method has been applied for fabricating uniaxially strained GeNWs [17, 18], the complex of this fabrication technique can be hardly suitable for monolithic integration in Si-based photonics and electronics. Additionally, the strain will release easily in free-standing NWs, whereas lateral GeNWs can accom-modate much high strain in themselves. Thus, epitaxially grown lateral GeNWs with high biaxial tensile strain are required for achieving direct bandgap transition as well as carrier mobility enhancement.

To date, dislocation-free and highly biaxial tensile-strained Ge quantum dots on InP (001) have shown potentials for direct bandgap emitting simulated by finite element method (FEM) [19]. Similar to this, in this work, we theoretically predict morphology of exposed surfaces and growth direction of biaxially tensile-strained GeNWs on a relaxed GaSb template that can be grown directly on Si with an AlSb buffer layer [16, 20]. We choose {110}, {105}, and {111} as exposed surfaces of lateral GeNWs and compare the total energy change in the steady-state system. We ignore the influence of dislocation and frac-ture [21] in this highly strained system for simplicity. The simulation based on FEM reveals that there exists a crit-ical amount of Ge. Below the critcrit-ical value, GeNWs are exposed by{105}, while above the critical value, they are exposed by {110}. Almost all the GeNW region can be converted into direct bandgap, which is the difference of the conduction band minima and the light hole band max-ima at the-point. Besides, we also qualitatively analyze the change of strain-dependent carrier effective mass at the-point to indirectly predict the enhancement in both electron and hole mobility.

**Methods**

Lateral NWs normally reveal a triangle shape of cross section [22, 23]. Thanks to the 1D property of NW shown in Fig. 1a, an finite NW model similar to Zhang et al. in the supplemental material of Ref. [13] can be properly used for simulation in which both beginning and ending surfaces are fixed shown in Fig. 1b. Because of the boundary effect, we only discuss the center part of the NW and consider that the cross section of this part represents the situa-tion in an infinitively long NW. FEM is used to simulate distribution of tensile strain in GeNW with 7.7% lattice mismatch to GaSb. We calculate the total system energy increment after depositing the same amount of Ge in steady state in three situations: (i) [100] growth direction

with{110}facets exposed (situation A), (ii) [100] growth direction but with{105}facets exposed (situation B), and (iii) [110] growth direction with{111}facets exposed (sit-uation C). The cross sections of these three sit(sit-uations are shown in Fig. 1c. The areas of cross section are kept the same, representing equal amounts of Ge.

The total system energy change per unit length (J/nm) includes overall difference in strain energy, surface energy, and edge energy [24] and can be given by:

*E*total=*E*strain+*E*surface+*E*edge. (1)
The first term*E*strainrepresents the strain energy
differ-ence of the steady system before and after Ge deposition
and is expressed in unit volume,

*u*= 1

2*Y*

*i*=*j*

*τ*2

*ij*−

*ν*
*Y*

*i<j*

*τiiτjj*+

1
2*G*

*i<j*

*τ*2

*ij* (2)

where*τij*=*Cijεij*(*i, j*=1, 2, 3) denote the stress tensor,*Cij*

and*εij*are the elastic constants and strain tensor,

respec-tively,*Y*and*G*are the equivalent Young’s modulus and the
equivalent shear modulus, respectively, and*ν*is the
equiv-alent Poisson ratio. In the 2D cross section considered,
the total strain energy change can be obtained by
integrat-ing area with the value of*u*on every point. The second
term*E*surfaceis related to the difference of surface energy
before and after Ge deposition. The surface energy in the
cross section of our situations can be rewritten as [23]

*γi*=

2*h*

sin*θi(σi*−*σ(*001*)*

cos*θi)* (3)

where *h* is the height of the GeNW cross section, *σi*

(*i*=A, B, and C) is the average surface energy of the
exposed facets under unit area, and the corresponding
angel between the NW facets and interface is labeled by

*θi*as schematically shown in Fig. 1c. The strain in surface

energy can be neglected due to its slight impact as the treatment in Ref. [25]. Table 1 shows surface energy values from literature. The last term called edge energy change stands for the change of energy cost for forming sharp edges and is given by

*E*edge=3*Γ* (4)

where 3*Γ* is the total edge energy containing the top and
two basal facet intersections. The estimated value of 3*Γ*
is 3.7 eV/nm by experimental fitting [26] and the
influ-ence of the edge energy can be ignored due to the hardly
varied value [25]. Hence, it is valid to calculate the energy
increment of*E*total−3*Γ*.

After knowing the strain distribution, the strain-dependent conduction band decrement at the- and the L-valley can be calculated with neglecting the quantum effect. The conduction band of the -valley is lowered only with hydrostatic strain by

**Fig. 1**Schematics of GeNW on GaSb:**a**3D model,**b**simplified finite model, and**c**cross sections of GeNW with different facets

where*ac*denotes hydrostatic deformation potential with

the value of−8.24 eV at the -point [27], *εxx*, *εyy* and

*εzz* are the strain in *x*, *y,* and *z* direction in the

mate-rial coordinate system, respectively. However, the shift of the conduction band at the L-point is subject to both hydrostatic and shear strain [19], given by

*E _{c}*L=

*d*+

1
3*u*

*(εxx*+*εyy*+*εzz)*

−2
3*u*

|*εxy*| + |*εyz*| + |*εxz*|

(6)

where*d*and*u*are dilation deformation potential with

the value of −6.97 eV and uniaxial deformation poten-tial with the value of 16.3 eV at the L-valley, respectively. For converting Ge into a direct bandgap material, the -valley has to be lower than the L--valley, which means

*E*,L

*c* =*Ec*−*E*L*c* *<*−0.136 eV. Here, we use*E*DT=
*E*,L

*c* +0.136 to present the difference in the- and the

**Table 1**The average surface energy of different facets in Ge and

GaSb at 300 K

Material Facets Surface Energy (eV/nm2) Reference

Ge {110} 8.125a [34]

{105} 6.4b _{[14]}

{111} 6.625a _{[34]}

GaSb {100} 10a [35]

a_{The value from experiments}

b_{Theoretical results}

L-point. Once the -point descends below the L-point,

*E*DTwill be negative. A series of tensile-strained GeNWs
with varied sizes are simulated to show the direct bandgap
transition.

In addition, due to the high tensile strain in the GeNW, the-valley is below the L-valley while the light hole band maxima becomes the valence maxima [28]. The bandgap in such a high tensile-strained GeNW will be the differ-ence between the-valley and the light hole band maxima at the-point. Thus, the spatially distributed bandgap as well as the band edge energies at the -point which is

[image:3.595.56.291.637.714.2]both electron and hole mobility in a highly tensile-strained GeNW via the decrease of both electron and hole effective mass at the-point.

**Results and Discussions**

We consider the system is initially under full tensile strain
owing to the large lattice mismatch of 7.7% between Ge
and GaSb. Figure 2 shows the 2D residual strain
distri-bution including in-plane strain*εxx*, shear strain*εxy*, and

vertical strain *εzz* of situation A with the base width of

*w*= 40 nm for example in the steady state after relaxation.
The strain definition here is*(a*Ges−*a*Ge*) /a*Ge, where*a*Ges
and*a*Geare lattice constants of strained and relaxed Ge,
respectively. As seen in Fig. 2a,*εxx*has the maximum value

of about 15.4% at two basal edges which is much larger
than the initial strain, but decreases sharply from the edge
to the center with the minimum value of about 3.3%. In*z*
-direction from the bottom to the top of GeNW,*εxx*also

drops due to the relaxation of GeNW. The distribution
of*εzz*is found to have similar characteristics with*εxx* in

Fig. 2b. Unlike biaxial strain in Ge thin film, Fig. 2c shows
that the asymmetrically distributed shear strain
compo-nent of GeNW plays a significant role in direct bandgap
transition. The strain distribution is quite similar during
three situations. Nevertheless, the values of strain
com-ponents are different in three situations because of the
diverse width-height ratio (*W/H*) induced by its shape.
Situation B with GeNW exposed by{105}surfaces has the
largest*W/H*of 10, exhibiting high strain similar to that in
the Ge thin film. Situation C with{111}surfaces exposed
shows high strain as well since the NW growth
orienta-tion along the [110] remains an invariable value of strain,
raising the value of*εxx*and*εyy*simultaneously. Thus, the

in-plane strain can hardly be relaxed.

In accordance with the strain distribution, the strain energy increment can be obtained. As discussed previ-ously, situation B holds the highest strain energy incre-ment, while situation A has the lowest one. However, for the surface energy change, situation B gives decreas-ing negative values with increasdecreas-ing area of cross section and the other two situations reveal very close positive

values under the same area. The total energy increment
excluding edge energy change is shown in Fig. 3a. The
result shows that it is less likely to form GeNWs only
in situation C due to the energy increment never being
the lowest. There are two different consequences of the
energy increment with the increase of the area, and the
vertical dash line is marked to present the critical value
of area, A*c* = 136.2 nm2, which means the amounts of

Ge. When the area is less than 136.2 nm2, GeNWs are
inclined to form the shape in situation B, but in situation A
after depositing more Ge. The calculation result predicts
that tensile-strained GeNWs on GaSb may prefer to
form-ing high*W/H*triangle shape in cross section when a low
amount of Ge is deposited, whereas forming low *W/H*
one after exceeding the critical value. Figure 3b–e shows
the distributions of hydrostatic strain and the sum of
abso-lute value of shear strain components in situation A and B
under the critical area. Comparing situation A with B, in
spite of that situation A holds the greater maximum value
of both hydrostatic strain and|*εxy*| + |*εyz*| + |*εxz*|, situation

B has larger average hydrostatic strain but smaller
aver-age value of|*εxy*| + |*εyz*| + |*εxz*|. Meanwhile, situation B

demonstrates a small difference in spatial distribution of
both hydrostatic strain and|*εxy*|+|*εyz*|+|*εxz*|. These

prop-erties are very similar to Ge thin film and are attributed to
its high*W/H*value. As a result, referring to Eqs. (5) and
(6), situation B exhibits smaller value of*E*DTthan that of
situation A, leading to a high possibility to convert Ge into
a direct bandgap material.

Because of the high tensile strain in GeNW, nearly
all the region of GeNW can be converted into direct
bandgap. Figure 4a shows the distribution of*E*DTwith
increasing the size of GeNW. The value of *E*DTdrops
from the top to the bottom in GeNWs. Interestingly, the
minimum of*E*DT is located in the bottom edge of the
cross section in situation B, but in the bottom center in
sit-uation A. The reason of this different distribution is that
the significant shear strain at the bottom edge in
situa-tion A contributes more to*E*L* _{c}* than that in situation B.
For GeNW in situation B below the critical area, the
aver-age

*E*DTis much lower than that in situation A above

-0.02 0.02 0.06 0.10

z

x

**a**

-0.06 -0.04 -0.02 0 0.02

**b**

-0.006 -0.002 0.002 0.006

**c**

**Fig. 2**Residual strain distribution of a GeNW in situation A with the basal width of 40 nm:**a**x component strain*εxx*,**b**z component strain*εzz*, and**c**

**a**

**b**

**d**

**e**

**c**

0 0.05 0.10 0.15
[image:5.595.61.541.87.230.2]
0 0.04 0.08 0.12 0.01 0.03 0.05 0.07 0.09 0.02 0.04 0.06 0.08 0.10

**Fig. 3 a**The total energy change excluding the edge energy change 3vs. the cross section area (the*dash line*is the critical value of minima about

136.2 nm2_{in different situations).}_{b}_{–}_{e}_{hydrostatic strain and}_{|}_{ε}

*xy*| + |*εyz*| + |*εxz*|in**b**,**c**situation A and**d**,**e**situation B at the critical value

the critical area as shown in Fig. 4b. At the critical point,
the average of *E*DT suddenly rises from the value of
−0.308 to−0.137 eV. Furthermore, for the same shape,
the distribution and the average of *E*DT are basically
similar, without obvious relation to the size. In order to
discover the inherent relation to the strain in GeNW, we
plot the hydrostatic strain component at the GeNW base
with basal width in Fig. 5. The curves of hydrostatic strain
component with different sizes versus the relative
posi-tion of the base in a GeNW almost overlap except for the
difference in the peripheral region. The consistent
conse-quences are found in*εxx* and the sum of absolute shear

components. Thus, the strain-induced value of*E*DT
pos-sesses the identical distribution in GeNW with the same
shape.

Further, we simulate the strain-induced bandgap map-ping in the cross section of the 40-nm wide GeNW shown

in Fig. 6a. The spatial distribution of bandgap is derived
from the variable value of strain-dependent band edges
at the-point. Figure 6b exhibits the band edge energy
at -point along the*z*-direction of the GeNW. We find
that both the conduction band and the valence band edges
including the light hole band and the heavy hole band
change significantly in the first 15 nm and then slightly.
The tops of the light and the heavy hole band separate
and tend to shift in opposite directions with increasing
the tensile strain. From Fig. 6a, b, the bandgap
signifi-cantly increases in the first 15 nm to reach about 0.30 eV,
then changes slightly around a value of 0.24 eV, which is
the bandgap in the most GeNW regions. Since the light
hole band maxima is higher than that of the heavy hole
band at the -point in the GeNW, holes in the valence
band prefer to situating at the light hole band maxima.
Thus, the electron-hole recombination will occur between

A

rea in

cre

ase

**a**

**b**

DT

(eV)

**Fig. 4 a**The distribution of*E*DTwith increase of the area (the*color bar*denotes the value of*E*DT).**b**The average of*E*DTvs. the area. The critical

### Hydrostatic Strain

### x/w

**Fig. 5**Hydrostatic strain component at the base of GeNW vs. x/w

with different basal widths

the conduction band minimum and the light hole band maximum at the-point if we neglect the overlap of the space-dependent electron and hole wave functions. Inter-estingly, the light hole band maxima moves even above the conduction band minima in the region of the NW bot-tom marked as a black curve in Fig. 6a with hydrostatic strain more than ∼5.0%. The negative bandgap we cal-culate under highly tensile strain may cause complicated consequences such as semimetallic [31] or inverted [32] band structure.

Finally, the mobility of electrons and holes will be enhanced under such highly tensile strain in the GeNW. For relaxed Ge, the electron transport is mainly con-tributed by electrons domiciled in the L-valley. When Ge is under tensile strain so that the -valley is below the L-valley as shown in Fig. 3a, the primary contribution of electron transport is from the-valley. On the other hand, the dominant participation of holes in the trans-port is from the light hole band at the -point under

highly tensile strain, while the heavy hole band occupies
the valence band maxima in the relaxed case. Due to much
smaller electron effective mass at the-point than that at
the L-point, as well as the decreased effective mass from
the heavy hole band maxima to the light hole band
max-ima, the mobility of not only electrons but also holes can
be enhanced. The tensile strain can be theoretically
pre-dicted to reduce the effective mass of electrons and holes
at the -point in a model of quantum dot by*Califano*
and*Harrison*[29]. Although the quantitative calculation
method is unsuitable for our NW model, we qualitatively
assume that tensile strain can modify the effective mass
at **k** = 0 by increasing the curvature of dispersion
rela-tion for small**k**in the vicinity of the-point. Thus, the
mobility of both electrons and holes can be enhanced in
tensile-strained GeNWs. The splitting valence bands also
induce strong electron-phonon coupling and intraband
scattering [33], which limits the hole mobility to be lower
than the electron mobility.

**Conclusions**

In summary, we have proposed tensile-strained GeNWs
on GaSb, comparing three different situations via total
energy change before and after Ge deposition. The result
displays that the GeNW is inclined to form {105}
sur-faces along the100growth direction before the critical
amount, while exposed by{110} surfaces after the
criti-cal amount. The residual strain field and bandgap analysis
have shown that the same shape has the similar
distri-bution both in strain and *E*DT regardless of size.
Fur-thermore, the in-plane strain and the hydrostatic strain
reduce not only from the edges to the center but also from
the bottom to the top as well in all the situations. Due to
the high tensile strain, almost the entire GeNW on GaSb
can be converted into a direct bandgap material in the
two possible situations. Also, the light holes mainly
par-ticipate in the electron-hole recombination and electric

**b**

**a**

**Fig. 6 a**The strain-dependent bandgap in the GeNW distributed by positions.**b**The strain-dependent band edge energies along*z*direction in the

transport at the-point because the light hole band max-ima becomes the maxmax-ima of the valence band in highly tensile strain. The mobility of not only electrons but also holes can be enhanced owing to the decrease of the carrier effective mass at the-point determined by the tensile strain. The attractive performance predicted theoretically implies that tensile-strained GeNWs are promising to be applied to optoelectronics for light source and micro-electronics for high speed devices in Si-photonics and electronics, respectively.

**Acknowledgements**

This study was supported by the National Natural Science Foundation of China (61404153), the Shanghai Pujiang Program (14PJ1410600), the Key Research Program of the Chinese Academy of Sciences (KGZD-EW-804), and the Creative Research Group Project of Natural Science Foundation of China (61321492).

**Authors’ contributions**

ZZ did the simulation, analyzed the simulated data, and wrote the manuscript. YS proposed the idea and designed the model of the structure and the main simulation. QC, ZZ, LZ, and YL assisted in the simulation and the result discussions. SW supervised the work and revised the manuscript. All authors read and approved the final manuscript.

**Competing interests**

The authors declare that they have no competing interests.

**Publisher’s Note**

Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.

**Author details**

1_{State Key Laboratory of Functional Materials for Informatics, Shanghai}

Institute of Microsystem and Information Technology, Chinese Academy of
Sciences, Shanghai 200050, China.2_{School of Physical Science and}

Technology, ShanghaiTech University, Shanghai 201210, China.3_{University of}

Chinese Academy of Sciences, Beijing 100190, China.4_{Department of}

Microtechnology and Nanoscience, Chalmers University of Technology, 41296 Gothenburg, Sweden.

Received: 7 May 2017 Accepted: 19 July 2017

**References**

1. Lee ML, Leitz CW, Cheng Z, Pitera AJ, Langdo T, Currie MT, Taraschi G,
Fitzgerald EA, Antoniadis DA (2001) Strained ge channel p-type
metal-oxide-semiconductor field-effect transistors grown on si1−*xgex/si*
virtual substrates. Appl Phys Lett 79(20):3344–3346

2. Saraswat K, Chui CO, Krishnamohan T, Kim D, Nayfeh A, Pethe A (2006) High performance germanium MOSFETs. Mater Sci Eng: B 135(3):242–249 3. Fischetti MV, Laux SE (1996) Band structure, deformation potentials, and

carrier mobility in strained Si, Ge, and Sige alloys. J Appl Phys 80(4):2234–2252

4. Zhang F, Crespi VH, Zhang P (2009) Prediction that uniaxial tension along

111produces a direct band gap in germanium. Phys Rev Lett 102(15):156401

5. Niquet Y, Rideau D, Tavernier C, Jaouen H, Blase X (2009) Onsite matrix elements of the tight-binding hamiltonian of a strained crystal: application to silicon, germanium, and their alloys. Phys Rev B 79(24):245201 6. El Kurdi M, Fishman G, Sauvage S, Boucaud P (2010) Band structure and

optical gain of tensile-strained germanium based on a 30 band k·p formalism. J Appl Phys 107(1):013710

7. Yang Y, Ho W, Huang C, Chang S, Liu C (2007) Electron mobility enhancement in strained-germanium n-channel

metal-oxide-semiconductor field-effect transistors. Appl Phys Lett 91(10):102103

8. Pillarisetty R, Chu-Kung B, Corcoran S, Dewey G, Kavalieros J, Kennel H, Kotlyar R, Le V, Lionberger D, Metz M, et al (2010) High mobility strained germanium quantum well field effect transistor as the p-channel device option for low power (vcc=0.5 v) iii-v cmos architecture. In: Electron Devices Meeting (IEDM), 2010 IEEE International. IEEE. pp 6–7 9. Agarwal R, Lieber C (2006) Semiconductor nanowires: optics and

optoelectronics. Appl Phys A 85(3):209–215

10. Kamins T, Li X, Williams RS, Liu X (2004) Growth and structure of chemically vapor deposited ge nanowires on si substrates. Nano Lett 4(3):503–506 11. Lauhon LJ, Gudiksen MS, Wang D, Lieber CM (2002) Epitaxial core-shell and core-multishell nanowire heterostructures. Nature 420(6911):57–61 12. Xiang J, Lu W, Hu Y, Wu Y, Yan H, Lieber CM (2006) Ge/si nanowire

heterostructures as high-performance field-effect transistors. Nature 441(7092):489–493

13. Zhang JJ, Katsaros G, Montalenti F, Scopece D, Rezaev RO, Mickel C, Rellinghaus B, Miglio L, De FS, Rastelli A (2012) Monolithic growth of ultrathin ge nanowires on si(001). Phys Rev Lett 109(8):1–5 14. Scopece D, Montalenti F, Beck MJ (2012) Stability of ge on si (1 1 10)

surfaces and the role of dimer tilting. Phys Rev B 85(8):085312

15. Fang Y, Tolle J, Roucka R, Chizmeshya A, Kouvetakis J, D’Costa V, Me ´nndez
J (2007) Perfectly tetragonal, tensile-strained ge on ge1−*ysny*buffered si
(100). Appl Phys Lett 90(6):061915

16. Akahane K, Yamamoto N, Gozu S-i, Ohtani N (2004) Heteroepitaxial growth of gasb on si (001) substrates. J Cryst Growth 264(1):21–25 17. Süess M, Geiger R, Minamisawa R, Schiefler G, Frigerio J, Chrastina D, Isella

G, Spolenak R, Faist J, Sigg H (2013) Analysis of enhanced light emission from highly strained germanium microbridges. Nat Photonics 7(6):466–472

18. Greil J, Lugstein A, Zeiner C, Strasser G, Bertagnolli E (2012) Tuning the electro-optical properties of germanium nanowires by tensile strain. Nano Lett 12(12):6230–6234

19. Chen Q, Song Y, Wang K, Yue L, Lu P, Li Y, Gong Q, Wang S (2015) A new route toward light emission from ge: tensile-strained quantum dots. Nanoscale 7(19):8725–8730

20. Vajargah SH, Ghanad-Tavakoli S, Preston J, Kleiman R, Botton G (2013) Growth mechanisms of gasb heteroepitaxial films on si with an alsb buffer layer. J Appl Phys 114(11):113101

21. Callister WD, Rethwisch DG (2007) Materials science and engineering: an introduction vol. 7. Wiley, New York. pp. 208–223

22. Omi H, Ogino T (1997) Self-assembled Ge nanowires grown on Si (113). Appl Phys Lett 71(15):2163–2165

23. Zhang G, Tateno K, Gotoh H, Nakano H (2010) Parallel-aligned GaAs nanowires with110orientation laterally grown on [311] b substrates via the gold-catalyzed vapor-liquid-solid mode. Nanotechnology

21(9):095607

24. Liu Q, Moll N, Scheffler M, Pehlke E (1999) Equilibrium shapes and energies of coherent strained inp islands. Phys Rev B 60(24):17008 25. Moll N, Scheffler M, Pehlke E (1998) Influence of surface stress on the

equilibrium shape of strained quantum dots. Phys Rev B 58(8):4566 26. Chen G, Sanduijav B, Matei D, Springholz G, Scopece D, Beck M,

Montalenti F, Miglio L (2012) Formation of ge nanoripples on vicinal si 1110: From stranski-krastanow seeds to a perfectly faceted wetting layer. Phys Rev Lett 108(5):055503

27. Van de Walle CG (1989) Band lineups and deformation potentials in the model-solid theory. Phys Rev B 39(3):1871

28. Kurdi ME, Fishman G, Sauvage S, Boucaud P (2010) Band structure and optical gain of tensile-strained germanium based on a 30 band k·p formalism. J Appl Phys 107(1):013710

29. Califano M, Harrison P (2002) Composition, volume, and aspect ratio
dependence of the strain distribution, band lineups and electron
effective masses in self-assembled pyramidal in1−*xgaxas/gaas and*
sixge1−*x/si quantum dots. J Appl Phys 91(1):389–398*

30. Murphy-Armando F, Fahy S (2011) Giant enhancement of n-type carrier mobility in highly strained germanium nanostructures. J Appl Phys 109(11):113703

31. Veal TD, Mahboob I, McConville C (2004) Negative band gaps in dilute
innxsb1−*x*alloys. Phys Rev Lett 92(13):136801

33. Sau JD, Cohen ML (2007) Possibility of increased mobility in Ge-Sn alloy system. Phys Rev B 75(4):045208

34. Jaccodine R (1963) Surface energy of germanium and silicon. J Electrochem Soc 110(6):524–527